advertisement

Derivation of an Analytical Solution to a ReactionDiffusion Model for Autocatalytic Degradation and Erosion in Polymer Microspheres The MIT Faculty has made this article openly available. Please share how this access benefits you. Your story matters. Citation Ford Versypt, Ashlee N., Paul D. Arendt, Daniel W. Pack, and Richard D. Braatz. “Derivation of an Analytical Solution to a Reaction-Diffusion Model for Autocatalytic Degradation and Erosion in Polymer Microspheres.” Edited by Zhen Jin. PLoS ONE 10, no. 8 (August 18, 2015): e0135506. As Published http://dx.doi.org/10.1371/journal.pone.0135506 Publisher Public Library of Science Version Final published version Accessed Wed May 25 19:20:27 EDT 2016 Citable Link http://hdl.handle.net/1721.1/99884 Terms of Use Creative Commons Attribution Detailed Terms http://creativecommons.org/licenses/by/4.0/ RESEARCH ARTICLE Derivation of an Analytical Solution to a Reaction-Diffusion Model for Autocatalytic Degradation and Erosion in Polymer Microspheres Ashlee N. Ford Versypt1,2¤a, Paul D. Arendt1¤b, Daniel W. Pack1,3,4, Richard D. Braatz1,2* a11111 1 Department of Chemical and Biomolecular Engineering, University of Illinois at Urbana-Champaign, Urbana, Illinois, United States of America, 2 Department of Chemical Engineering, Massachusetts Institute of Technology, Cambridge, Massachusetts, United States of America, 3 Department of Chemical and Materials Engineering, University of Kentucky, Lexington, Kentucky, United States of America, 4 Department of Pharmaceutical Sciences, University of Kentucky, Lexington, Kentucky, United States of America ¤a Current address: School of Chemical Engineering, Oklahoma State University, Stillwater, Oklahoma, United States of America ¤b Current address: CNA, Chicago, Illinois, United States of America * braatz@mit.edu OPEN ACCESS Citation: Ford Versypt AN, Arendt PD, Pack DW, Braatz RD (2015) Derivation of an Analytical Solution to a Reaction-Diffusion Model for Autocatalytic Degradation and Erosion in Polymer Microspheres. PLoS ONE 10(8): e0135506. doi:10.1371/journal. pone.0135506 Editor: Zhen Jin, Shanxi University, CHINA Received: January 26, 2015 Accepted: July 22, 2015 Published: August 18, 2015 Copyright: © 2015 Ford Versypt et al. This is an open access article distributed under the terms of the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original author and source are credited. Data Availability Statement: All relevant data are within the paper. Funding: The authors acknowledge the support of the National Institutes of Health (NIBIB 5RO1EB005181) and the National Science Foundation (Grant #0426328). A. N. Ford Versypt acknowledges the support of the U.S. Department of Energy Computational Science Graduate Fellowship Program of the Office of Science and National Nuclear Security Administration in the Department of Energy under contract DE-FG02-97ER25308. Abstract A mathematical reaction-diffusion model is defined to describe the gradual decomposition of polymer microspheres composed of poly(D,L-lactic-co-glycolic acid) (PLGA) that are used for pharmaceutical drug delivery over extended periods of time. The partial differential equation (PDE) model treats simultaneous first-order generation due to chemical reaction and diffusion of reaction products in spherical geometry to capture the microsphere-sizedependent effects of autocatalysis on PLGA erosion that occurs when the microspheres are exposed to aqueous media such as biological fluids. The model is solved analytically for the concentration of the autocatalytic carboxylic acid end groups of the polymer chains that comprise the microspheres as a function of radial position and time. The analytical solution for the reaction and transport of the autocatalytic chemical species is useful for predicting the conditions under which drug release from PLGA microspheres transitions from diffusion-controlled to erosion-controlled release, for understanding the dynamic coupling between the PLGA degradation and erosion mechanisms, and for designing drug release particles. The model is the first to provide an analytical prediction for the dynamics and spatial heterogeneities of PLGA degradation and erosion within a spherical particle. The analytical solution is applicable to other spherical systems with simultaneous diffusive transport and first-order generation by reaction. PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 1 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model Competing Interests: The authors have declared that no competing interests exist. Introduction Poly(D,L-lactic-co-glycolic acid) (PLGA) microspheres are biodegradable polymeric devices that are widely studied for controlled-release drug delivery [1–4]. Compared to conventional drug dosage forms, controlled-release drug delivery can provide enhanced control of drug concentrations and biodistribution, reduce side effects, and improve patient compliance. Drug molecules dispersed in the bulk polymer are released by diffusion by two main pathways: through the nondegraded polymer bulk and through aqueous pores that form in the polymer bulk as the polymer undergoes hydrolysis. Between microsphere size range extremes, drug release may transition from the diffusion-controlled regime (diffusive release through the nondegraded polymer bulk is faster through smaller microspheres that have shorter diffusion lengths than in larger microspheres) to the erosion-controlled regime (diffusive release through aqueous pores is faster through larger microspheres that have eroded porous interiors than in smaller microspheres). The drug release rates for drug molecules with different sizes and water solubilities depend strongly on the release regimes. Small, poorly water-soluble molecules are known to diffuse more easily through the nondegraded polymer bulk so are released more quickly in the diffusion-controlled regime [5, 6]. Conversely, small, highly water-soluble molecules and macromolecules are known to diffuse more easily through aqueous pores so are released more quickly in the erosion-controlled regime [7]. Thus, drug release is coupled to polymer degradation by the dynamics and spatial distribution of developing pores. To describe the development of the pore structure in the microspheres, it is first necessary to consider how the polymer reacts and forms pores. PLGA degrades chemically by acid-catalyzed ester hydrolysis in the polymer bulk rather than from the surface inward because the water penetrates into the polymer matrix faster than the rate of hydrolysis [8]. The carboxylic acid end groups of the PLGA polymer chains can donate protons to autocatalyze the hydrolytic degradation, which accelerates the reaction kinetics. The amount of autocatalyst increases as polymer chains are broken to produce smaller chains because each of the smaller chains includes an autocatalytic end group. Small polymer fragments up to and including nonamers are water-soluble [9–11]. The water-soluble fragments dissolve in water and diffuse out of the polymer through water-filled pores, which leads to polymer erosion (mass loss) and increases pore volume in the microspheres. Autocatalytic hydrolysis is more substantial in the interior of large microspheres where the diffusion of degradation products is limited, leading to accumulation of acidic polymer end groups [7, 12–14]. Although many models have been proposed for drug release from PLGA microspheres [15– 18], the mathematical formulation needed to accurately predict microsphere-size-dependent drug release is still unclear [18, 19]. Here, we focus on the clarifying the complex effects of autocatalysis on simultaneous polymer degradation and erosion in microspheres of different sizes. By considering the polymer in isolation without encapsulated drug molecules, we aim to contribute to the understanding of the development of porous domains in the microspheres, which can then be used incorporated into future models that include drug transport to describe the entire process of drug release from these types of dynamic porous materials. The autocatalytic PLGA degradation reaction has been modeled previously [20, 21]; however, the models treated homogeneous degradation before the start of erosion, and the analytical solutions of the models do not depend on the microsphere size or spatial heterogeneities within the microspheres. Models using reaction-diffusion equations have been applied to a comparable drug delivery system: covalently bonded polymer-drug conjugates in solid polymers. The models included first-order cleavage of polymer-drug bonds followed by diffusive release of drug from polymer matrices [22, 23]. While the models for the polymer-drug conjugates treated a drug delivery system involving reaction and diffusion, the models cannot be PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 2 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model applied directly to PLGA because the reaction kinetics in those models were independent of the drug diffusion dynamics. The reaction and diffusion processes for PLGA microspheres are coupled and should not be treated independently. A reaction-diffusion model has been proposed previously [24] to treat autocatalytic degradation and erosion in the polymer plates and cylinders composed of chemically similar poly (lactic acid) (PLA), and the numerical predictions were compared to experimental data from a study on the degradation of PLA plates of different thicknesses [25]. While the model in [24] can be extended to other geometries using finite element analysis to solve the equations numerically, the influence of the relationship between diffusion and reaction parameters on the zones where diffusion and degradation have strong or weak influences was only presented for onedimensional planar and cylindrical geometries. We aim to derive an analytical solution to a reaction-diffusion model specifically for the case of spherical geometry that can assess the relative dominance of the reaction and diffusion phenomena through a single dimensionless parameter. Reaction-diffusion equations have commonly been used to model spherical catalyst pellets that experience simultaneous reaction and diffusion, and analytical solutions to the equations are available [26, 27]. Despite the similarities in the reaction-diffusion equations for the two systems, the catalyst pellets and PLGA microspheres differ in ways that are critical for their mathematical treatment: (1) the reaction term in PLGA is a generation term instead of a consumption term and (2) the directions of diffusion are reversed for PLGA microspheres and catalyst pellets. In catalyst pellets, the reactant diffuses into the sphere where it is consumed by a reaction. In contrast, the autocatalytic carboxylic acid end groups in PLGA microspheres are distributed throughout the sphere where more are generated by the degradation reaction, and some fraction of the autocatalyst diffuses out of the sphere. These differences between the physics of reaction and diffusion in spherical catalyst pellets and PLGA microspheres must be carefully accounted for during the analogous mathematical analyses of the reaction-diffusion equations used to model the systems. Here, we derive an analytical expression for the transient, radial concentration of the autocatalytic carboxylic acid end groups of PLGA by simultaneously treating degradation and erosion of the polymer. Quantifying the transient, spatial distribution of the autocatalyst within the polymer is important for understanding how different conditions may contribute to accelerating hydrolysis in the interior of large microspheres and for preventing adverse effects of the acidic conditions within a microsphere on the drug stability or bioactivity [28]. Additionally, such a mathematical treatment provides insights into how the coupling between autocatalysis and drug diffusion may trigger transitions between diffusion-controlled and erosion-controlled drug release regimes. Methods Mathematical model for the autocatalyst concentration The conservation equation for a chemical species subject to reaction and diffusion within a radially symmetric sphere is @c 1 @ 2 D @c ¼ r 2 þ RV ; ð1Þ @t r2 @r R @r where c(r, t) is the concentration, 0 r 1 is the normalized radial position deﬁned as r ¼ ^r =R, ^r is the the radial distance from the center of the sphere, R is the radius of the sphere, t 0 is time, D is the diffusion coefﬁcient, and RV is the net rate of generation of species per volume. We assume that the microsphere volume is constant for bulk-eroding PLGA, PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 3 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model neglecting any effects of possible microsphere swelling. The chemical species of interest is the autocatalytic carboxylic acid end groups of the polymer chains or autocatalyst. PLGA degradation is often treated with pseudo-ﬁrst-order kinetics [13, 18], where the autocatalyst undergoes ﬁrst-order growth while the concentrations of water, cH2O and ester bonds in the polymer, cE, are assumed to remain constant, giving RV ¼ kc; ð2Þ where the rate constant k for random ester bond hydrolysis incorporates the constant concentrations cH2O and cE (the applicability of the assumption of constant cE is checked in the Results and discussion section). PLGA erosion is treated by assuming that all carboxylic acid end groups have a uniform constant diffusion coefﬁcient D independent of the length of the polymer chain to which they are attached; with this assumption, diffusion of degradation products can be included in the analytical expression for autocatalyst concentration. Substituting α = D/R2 and (Eq 2) into (Eq 1) yields @c a @ 2 @c ¼ r þ kc: ð3Þ @t r2 @r @r for k > 0, and α > 0. The boundary conditions are @cð0; tÞ ¼ 0; @r t0 ð4Þ cð1; tÞ ¼ cr1 ; t 0; ð5Þ and and the initial concentration distribution is cðr; 0Þ ¼ ct0 ðrÞ; 0 r < 1; ð6Þ where cr1 0 and ct0 > 0. Note that cr1 ct0 for ﬂux toward the exterior of the sphere. Analytical solution for the autocatalyst concentration By substituting v(r, t) = rc(r, t), the partial differential equation (PDE) (Eq 3) and its initial and boundary conditions are transformed to a linear, nonhomogeneous second-order PDE with a source term and nonhomogeneous Dirichlet boundary conditions: @v @2v ¼ a 2 þ kv; @t @r ð7Þ with boundary conditions vð0; tÞ ¼ 0; t0 ð8Þ vð1; tÞ ¼ cr1 ; t0 ð9Þ and and initial condition vðr; 0Þ ¼ rct0 ðrÞ; PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 0 r < 1: ð10Þ 4 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model The PDE for v(r, t) can be solved by superposition of the solutions to two related problems [29]: (i) the complementary steady-state boundary value problem, 0¼a d2 u þ ku dr 2 ð11Þ with boundary conditions u(0) = 0 and u(1) = cr1, where u(r) is the equilibrium steady-state distribution, and (ii) the PDE for the function w(r, t) v(r, t) − u(r), @w @2w ¼ a 2 þ kw @t @r ð12Þ with homogeneous boundary conditions wð0; tÞ ¼ wð1; tÞ ¼ 0; t0 ð13Þ and initial condition wðr; 0Þ ¼ rct0 ðrÞ uðrÞ; 0 < r < 1: ð14Þ The steady-state solution, u(r), and the solution to (Eq 12) for w(r, t) by the method of eigenfunction expansion are derived below and then combined to obtain the solutions for v(r, t) and c(r, t). Steady-state solution for u(r). The steady-state boundary value problem (Eq 11) can be rewritten as 0¼ d2 u þ F2 u; dr 2 ð15Þ 0 r 1; where the Thiele modulus, F, for this ﬁrst-order reaction-diffusion system is pﬃﬃﬃﬃﬃﬃﬃﬃ F ¼ k=a: ð16Þ The Thiele modulus characterizes the relative importance of diffusion and reaction and is deﬁned as the ratio of the characteristic times for diffusion (1/α) and reaction in the absence of mass transfer limitations (1/k). The solution is of the form [30] u ¼ A cos ðFrÞ þ B sin ðFrÞ: ð17Þ The boundary condition u(0) = 0 for ﬁnite values of c requires that A = 0. At the surface, uð1Þ ¼ cr1 ¼ B sin F; ð18Þ so B = cr1/ sinF. The solution to the steady-state ordinary differential equation (ODE) with nonhomogeneous boundary conditions is uðrÞ ¼ rcðrÞ ¼ cr1 sin ðFrÞ : sin F ð19Þ Method of eigenfunction expansion solution for w(r, t). The linear, nonhomogeneous PDE with homogeneous boundary conditions given by (Eq 12) can be solved using the method of eigenfunction expansion [29], which consists of expanding the unknown solution w(r, t) in a series of the eigenfunctions for the related homogeneous problem: wðr; tÞ ¼ 1 X an ðtÞn ðrÞ; ð20Þ n¼1 PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 5 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model where an(t) are the time-dependent, generalized Fourier coefﬁcients and ϕn(r) are the eigenfunctions of the homogeneous PDE for diffusion without a source term with homogeneous Dirichlet boundary conditions, n ðrÞ ¼ sin ðnprÞ: ð21Þ The eigenfunction expansion of the source term is kwðr; tÞ ¼ 1 X bn ðtÞn ðrÞ; ð22Þ n¼1 where bn(t) = kan(t) since the source term is ﬁrst-order in the linearized concentration. The Fourier sine series can be differentiated term by term since w(r, t) and sin(nπr) satisfy the same boundary conditions [29]. Inserting the eigenfunction expansions for w(r, t) from (Eq 20) and the source term from (Eq 22) into the PDE in (Eq 12) yields 1 X da n¼1 n dt n ¼ 1 X ðan2 p2 Þan n þ 1 X kan n : n¼1 ð23Þ n¼1 For each n = 1, 2, . . ., dan da þ ðan2 p2 kÞan ¼ n þ n2 p2 F2 aan ¼ 0: dt dt ð24Þ The solution to (Eq 24) is an ðtÞ ¼ an ð0Þ exp ððn2 p2 F2 ÞatÞ; ð25Þ where the an(0) can be derived by multiplying (Eq 20) by ϕm for t = 0, considering the orthogonality of the eigenfunctions, and integrating over the spatial domain to give R1 wðr; 0Þ dr an ð0Þ ¼ 0 R 1 2 n n dr 0 Z 1 ð26Þ ¼ 2 ðvðr; 0Þ uÞ sin ðnprÞdr 0 Z ¼ 1 0 2rct0 ðrÞ sin ðnprÞdr þ 2cr1 npð1Þ n n2 p2 F2 In the speciﬁc case of uniform initial distribution, ct0(r) = ct0 and 2ct0 ð1Þ 2cr npð1Þ þ 21 2 an ð0Þ ¼ : np n p F2 n n ð27Þ Substituting the expressions for ϕn from (Eq 21), an from (Eq 25), and an(0) from (Eq 26) into (Eq 20) yields the solution to the nonhomogeneous PDE with homogeneous boundary conditions (Eq 12): n 1 Z 1 X 2cr npð1Þ 2rct0 ðrÞ sin ðnprÞdr þ 21 2 wðr; tÞ ¼ n p F2 ð28Þ 0 n¼1 exp ððn2 p2 F2 ÞatÞ sin ðnprÞ: Solution for v(r, t). Substituting the expressions for u from (Eq 19) and w from (Eq 28) into v = u+w yields the solution to the nonhomogeneous PDE with nonhomogeneous boundary PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 6 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model conditions (Eq 7): vðr; tÞ ¼ cr1 sin ðFrÞ sin F n 1 Z 1 X 2cr npð1Þ 2rct0 ðrÞ sin ðnprÞdr þ 21 2 þ n p F2 0 n¼1 ð29Þ exp ððn2 p2 F2 ÞatÞ sin ðnprÞ: Solution for c(r, t). The concentration of the autocatalyst in radial coordinates is v c¼ : r ð30Þ The indeterminate form at r = 0 is resolved by lim r!0 sin ðxrÞ ¼ lim x cos ðxrÞ ¼ x; r!0 r ð31Þ where x denotes a constant. The autocatalyst concentration at r = 0 is cð0; tÞ ¼ cr1 F sin F Z 1 ð32Þ n 1 X 2cr1 npð1Þ 2 2 2 exp ððn p F ÞatÞ; 2rct0 ðrÞ sin ðnprÞdr þ 2 2 þ np n p F2 0 n¼1 and at 0 < r < 1 is cðr; tÞ ¼ cr1 sin ðFrÞ r sin F n 1 Z 1 X 2cr npð1Þ 2rct0 ðrÞ sin ðnprÞdr þ 21 2 þ n p F2 0 n¼1 exp ððn2 p2 F2 ÞatÞ ð33Þ sin ðnprÞ : r With uniform initial distribution, (Eq 32) and (Eq 33) become cr1 F sin F 1 X cr1 n2 p2 n ct0 ð1Þ exp ððn2 p2 F2 ÞatÞ þ2 2 p2 F2 n n¼1 ð34Þ cr1 sin ðFrÞ r sin F 1 X c t0 cr1 np sin ðnprÞ n ð1Þ exp ððn2 p2 F2 ÞatÞ : þ2 2 2 2 np r n p F n¼1 ð35Þ cð0; tÞ ¼ and cðr; tÞ ¼ PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 7 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model Numerical solution for the autocatalyst concentration The partial differential equation for the autocatalyst concentration Eqs (3)–(6) can also be solved by numerical methods. The method of lines [31, 32] reduces the PDE to a system of ODEs by discretizing the radial dimension onto a finite grid with equal spacing Δr and coordinates ri = iΔr for i = 0, 1, . . ., N. Using the boundary conditions and the second-order centered finite difference approximations for spherical coordinates [33] to approximate the spatial derivatives, the semi-discrete ODE for the concentration at each grid point, ci(t), is 8 6a > > if i ¼ 0; > > Dr2 ðc1 c0 Þ þ kc0 ; > > < dci ð36Þ ¼ 0 if i ¼ N; dt > > > > > a > : ði þ 1Þciþ1 2ici þ ði 1Þci1 þ kci ; otherwise: 2 iDr The system of ODEs was solved using the function ode45 in MATLAB. The numerical solution gives suitable accuracy when compared with the analytical solution. Results and Discussion Transient autocatalyst profiles Our analytical expressions for the transient radial concentration of the autocatalyst Eqs (32)– (35) quantify the importance of the Thiele modulus, F, for determining whether PLGA degradation and erosion are enhanced by accumulation or diminished by diffusion. The results presented here are all for the case of uniform initial distribution ct0(r) = ct0 given by Eqs (34)–(35). For small values of F (Fig 1a-1b), diffusion dominates the conservation equation, so any amount of the autocatalyst generated by the reaction diffuses away quickly and a steady state can be reached. Such a microsphere experiences homogeneous erosion without substantiallycatalyzed degradation (Fig 2a). Small microspheres, fast diffusion, or slow reaction can give small values of F. For intermediate values of F on the order of π (Fig 1c-1d), the autocatalyst accumulates in the center of the microsphere forming a hollow interior (Fig 2b). For large values of F (Fig 1e), the first-order reaction generation dominates the conservation equation, so the autocatalyst accumulates in the interior faster than it can diffuse from the sphere. Autocatalytic degradation is severe throughout the microsphere (Fig 2c), and the entire particle may erode rapidly. The predicted autocatalyst concentration profiles (Fig 1) and the illustrations of the spatial distribution of the autocatalyst in microspheres of different sizes where small sizes correspond to small values of F (Fig 2) are consistent with experimental visual evidence of the microspheres-size-dependent spatial distribution of the acidic microclimate within degrading PLGA microspheres [34]. Transition between regimes To assess the bounds on the concentration profiles in different ranges of F, the maximum values of the concentration profiles, which occur at the microsphere center r = 0, are compared (Figs 3 and 4). The upper and lower bounds are the reaction-dominant limit and the diffusiondominant limit, respectively. Considering only the degradation reaction without diffusion, the autocatalyst concentration is described by @crxn ¼ kcrxn ; @t PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 ð37Þ 8 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model Fig 1. Dimensionless autocatalyst concentration profiles. Autocatalyst concentration c/ct0 profiles as functions of the characteristic time (αt for Thiele modulus Φ π and kt for Φ > π) and dimensionless position r for cr1 = 0: (a) Φ = 0.1π, (b) Φ = 0.75π (c) Φ = π, (d) Φ = 1.25π, (e) Φ = 5π. The vertical axes of the plots are shown at different scales to zoom in on the full range of change in c/ct0 over the time period. The coloring is consistent between the plots to facilitate comparisons. doi:10.1371/journal.pone.0135506.g001 Fig 2. Sketch of spatial distribution of the autocatalyst in microsphere cross-sections in different ranges of Thiele modulus. (a) diffusion throughout for Thiele modulus Φ < < π, (b) diffusion near edges and accumulation/enhanced degradation in the center for Φ π, (c) accumulation/enhanced degradation throughout for Φ > > π. The autocatalyst is illustrated in white, and the polymer bulk is shown in black. doi:10.1371/journal.pone.0135506.g002 which has the solution crxn ðr; tÞ ¼ ct0 exp ðktÞ; ð38Þ where crxn is referred to as the reaction-dominant limit. This limit is the commonly treated case for autocatalytic hydrolysis kinetics [13], where the concentration at each position is independent of its neighbors. As F ! 1, c(r, t) ! crxn(t) (Fig 3), so values in the range F π are in the erosion-controlled regime. PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 9 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model Fig 3. Dimensionless autocatalyst concentration profiles at r = 0 for large Thiele modulus values. Autocatalyst concentration c/(ct0+cE) profiles at r = 0 as functions of time scaled by the maximum reaction time tmax for cr1 = 0 and large values of Thiele modulus Φ: Φ = π (red open circles), Φ = 1.25π (blue solid diamonds), Φ = 1.5π (green solid squares), Φ = 1.75π (black solid triangles), Φ = 2π (red solid circles), Φ = 2π (blue open diamonds), Φ = 3π (green open squares), Φ = 5π (black open triangles). The solution approaches the reaction-dominant limit crxn (red solid curve) as Φ ! 1. doi:10.1371/journal.pone.0135506.g003 Fig 4. Dimensionless autocatalyst concentration profiles at r = 0 for intermediate Thiele modulus values. Autocatalyst concentration c/ct0 profiles at r = 0 as functions of the characteristic time for diffusion for cr1 = 0 and intermediate values of Thiele modulus Φ: Φ = 0.25π (red open triangles), Φ = 0.5π (blue open circles), Φ = 0.75π (green open diamonds), Φ = 0.9π (black open squares), Φ = 0.99π (red solid triangles), Φ = π (blue solid circles). The solutions are bounded by the diffusion-dominant limit cdiffn (black dotted curve) as Φ ! 0 and the reaction-dominant limit crxn (red solid curve) as Φ ! 1. doi:10.1371/journal.pone.0135506.g004 PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 10 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model In a PLGA microsphere, the degradation reaction cannot continue infinitely because the hydrolysis reaction only proceeds as long as ester bonds can be cleaved in the polymer. The maximum time for the reaction occurs when all of the ester bonds have been converted to monomers, so crxn(r, tmax) = ct0 + cE and t max ¼ 1 ct0 þ cE 1 Mn0 ln ¼ ln ; ct0 M1 k k ð39Þ where Mn0 is the initial number-average molecular weight and M1 is the average weight of a monomer. As t ! tmax the assumption of constant ester bond concentration is violated. At t = 1/k, t/tmax 1–2% for PLGA 50:50 with M1 = 65.05 Da, Mn0 = 10–1000 kDa, and k = 0.012–0.08 day−1 [7], thus the constant ester concentration assumption is valid within the characteristic time for the reaction (kt = 1 gives t 12–80 days). Considering only diffusion without the degradation reaction, the autocatalyst concentration is described by @cdiffn @2c ¼ a diffn ; @t @r 2 ð40Þ with boundary and initial conditions given by Eqs (5)–(6), which has the solution [33] for r = 0 cdiffn ð0; tÞ ¼ cr1 þ 2ðcr1 ct0 Þ 1 X n ð1Þ exp ðn2 p2 atÞ ð41Þ n¼1 and for 0 < r < 1 cdiffn ðr; tÞ ¼ cr1 þ n 1 2ðcr1 ct0 Þ X ð1Þ exp ðn2 p2 atÞ sin ðnprÞ; pr n n¼1 ð42Þ where cdiffn is referred to as the diffusion-dominant limit. As F ! 0, c(r, t) ! cdiffn(r, t) (Fig 4), so values in the range F < π are in the diffusion-controlled regime. For intermediate values of F, the autocatalyst concentration is bounded by the diffusion- and reaction-dominant limits; the concentration peaks due to early accumulation and enhanced degradation in the center and later decays due to diffusion. F = π is the tipping point between the diffusion- and erosion-controlled regimes characterized by exponential decay and exponential growth of the autocatalyst, respectively. Steady-state autocatalyst profiles The autocatalyst concentration, c(r, t), exhibits exponential growth due to the first-order hydrolysis reaction and exponential decay due to diffusion. The steady-state limit is approached as the rates of diffusion and generation by reaction offset each other or when the reacting species has diffused out of the system completely. For the concentration to reach a steady state, the time derivative of c(r, t) must be zero; either the exponential term must (i) be constant or (ii) approach 0 as t ! 1. Therefore, n2 p2 F2 0; n ¼ 1; 2; . . . : ð43Þ In the most restrictive case of n = 1, F π. The constant surface boundary condition cr1 determines the magnitude of the diffusion driving force and indicates the concentration of species in the medium assuming no mass transfer limitations at the surface; this is consistent with a buffered medium where the autocatalyst released from the microsphere is perfectly absorbed by the medium. If cr1 = 0, values of F < π PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 11 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model Fig 5. Steady-state dimensionless autocatalyst concentration profiles. Steady-state dimensionless autocatalyst concentration lim cðr; tÞ=cr1 proﬁles as t!1 functions of dimensionless position r for boundary condition cr1 > 0 and Thiele modulus Φ < π: Φ = 0.25π (red open triangles), Φ = 0.5π (blue open circles), Φ = 0.75π (green open diamonds), Φ = 0.9π (black open squares). At r = 0, c/cr1 ! 1 as Φ ! π. doi:10.1371/journal.pone.0135506.g005 have trivial steady-state solutions c(r, t)/ct0 ! 0 as t ! 1 where the species diffuses completely out of the sphere preventing runaway of the first-order, autocatalytic reaction, while F = π has a stable nontrivial solution c(r, t)/ct0 ! 2 as t ! 1, balancing the contributions from the reaction and diffusion. If cr1 > 0, the steady-state solutions for F = mπ are nontrivial (Fig 5), and neither the steady-state linearized solution, u, nor the analytical solution, c, are defined for F = mπ, m = 1, 2, . . .. The transient profiles for F = mπ can be approximated by the numerical solution even though steady-state solutions do not exist in these cases. The case of cr1 > 0 is interesting from a mathematical perspective but may only be physically appropriate for media that have high concentrations of strong acid that augment the carboxylic acid end groups in catalyzing the degradation. The boundary condition cr1 = 0 is valid assuming no autocatalyst in a weakly acidic buffered medium and is used for the results shown in Figs 1, 3, and 4. Conclusions An analytical expression was derived for the transient, radial concentration of a species undergoing simultaneous diffusion and first-order reaction generation with constant, but not necessarily zero, surface boundary concentration. The expression differs from the common reaction-diffusion case treated in the spherical catalyst literature as we treat a generation rather than consumption reaction term. To our knowledge, this is the first application of such an analytical expression for the reaction-diffusion equation to PLGA microspheres to model degradation and erosion of the polymer. Treating the diffusive transport of the autocatalytic species to capture spatial heterogeneities during degradation is a unique contribution of this work. A limitation of the analytical expression for the autocatalyst concentration is the assumption that the diffusion coefficient is independent of the lengths of the polymer chains to which the autocatalytic carboxylic acid end groups are attached. In reality only a fraction of the polymer chains are small enough to be water-soluble and able to diffuse through the aqueous pores. To account for the overestimation of autocatalyst mobility in the assumption needed to simplify PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 12 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model the mathematical formulation, a smaller value for the diffusion coefficient than the value for just the soluble chains should be used to represent the average diffusivity of soluble and insoluble polymer chains. A more detailed model distinguishing between the diffusivities of soluble and insoluble autocatalyst populations would require a numerical solution to the PDE for each population. The analytical expression for autocatalyst concentration indicates that the Thiele modulus is a key parameter for predicting the transition between the diffusion- and erosion-controlled release regimes. With the coupling between reaction and diffusion of the autocatalyst treated by this model, size-dependent effects on autocatalysis can be explored and incorporated into detailed predictive models for drug delivery from autocatalytic PLGA microspheres, which could ultimately contribute to the in silico optimal design of controlled drug release particles. Author Contributions Conceived and designed the experiments: ANFV PDA DWP RDB. Performed the experiments: ANFV PDA. Analyzed the data: ANFV RDB. Contributed reagents/materials/analysis tools: ANFV PDA RDB. Wrote the paper: ANFV PDA DWP RDB. References 1. Edlund U, Albertsson AC. Degradable polymer microspheres for controlled drug delivery. Adv Polym Sci. 2002; 157:67–112. doi: 10.1007/3-540-45734-8_3 2. Sinha VR, Trehan A. Biodegradable microspheres for protein delivery. J Control Release. 2003; 90 (3):261–280. doi: 10.1016/S0168-3659(03)00194-9 PMID: 12880694 3. Freiberg S, Zhu XX. Polymer microspheres for controlled drug release. Int J Pharm. 2004; 282(1–2):1– 18. doi: 10.1016/j.ijpharm.2004.04.013 PMID: 15336378 4. Varde NK, Pack DW. Microspheres for controlled release drug delivery. Expert Opin Biol Ther. 2004; 4 (1):35–51. doi: 10.1517/14712598.4.1.35 PMID: 14680467 5. Berkland C, King M, Cox A, Kim K, Pack DW. Precise control of PLG microsphere size provides enhanced control of drug release rate. J Control Release. 2002; 82(1):137–147. doi: 10.1016/S01683659(02)00136-0 PMID: 12106984 6. Raman C, Berkland C, Kim K, Pack DW. Modeling small-molecule release from PLG microspheres: Effects of polymer degradation and nonuniform drug distribution. J Control Release. 2005; 103(1):149– 158. doi: 10.1016/j.jconrel.2004.11.012 PMID: 15773062 7. Berkland C, Pollauf E, Raman C, Silverman R, Kim K, Pack DW. Macromolecule release from monodisperse PLG microspheres: Control of release rates and investigation of release mechanism. J Pharm Sci. 2007; 96(5):1176–1191. doi: 10.1002/jps.20948 PMID: 17455338 8. Göpferich A. Mechanisms of polymer degradation and erosion. Biomaterials. 1996; 17(2):103–114. doi: 10.1016/0142-9612(96)85755-3 PMID: 8624387 9. Batycky RP, Hanes J, Langer R, Edwards DA. A theoretical model of erosion and macromolecular drug release from biodegrading microspheres. J Pharm Sci. 1997; 86(12):1464–1477. doi: 10.1021/ js9604117 PMID: 9423163 10. Van Nostrum CF, Veldhuis TFJ, Bos GW, Hennink WE. Hydrolytic degradation of oligo(lactic acid): A kinetic and mechanistic study. Polymer. 2004; 45(20):6779–6787. doi: 10.1016/j.polymer.2004.08.001 11. Kulkarni A, Reiche J, Lendlein A. Hydrolytic degradation of poly(rac-lactide) and poly[(rac-lactide)-coglycolide] at the air-water interface. Surf Interface Anal. 2007; 39(9):740–746. doi: 10.1002/sia.2580 12. Vert M, Li S, Garreau H, Mauduit J, Boustta M, Schwach G, et al. Complexity of the hydrolytic degradation of aliphatic polyesters. Angew Makromol Chem. 1997; 247:239–253. doi: 10.1002/apmc.1997. 052470116 13. Siepmann J, Elkharraz K, Siepmann F, Klose D. How autocatalysis accelerates drug release from PLGA-based microparticles: A quantitative treatment. Biomacromolecules. 2005; 6(4):2312–2319. doi: 10.1021/bm050228k PMID: 16004477 14. Klose D, Siepmann F, Elkharraz K, Siepmann J. PLGA-based drug delivery systems: Importance of the type of drug and device geometry. Int J Pharm. 2008; 354(1–2):95–103. doi: 10.1016/j.ijpharm.2007. 10.030 PMID: 18055140 PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 13 / 14 Analytical Solution to Polymer Microsphere Reaction-Diffusion Model 15. Siepmann J, Göpferich A. Mathematical modeling of bioerodible, polymeric drug delivery systems. Adv Drug Delivery Rev. 2001; 48(2–3):229–247. doi: 10.1016/S0169-409X(01)00116-8 16. Lao LL, Peppas NA, Boey FYC, Venkatraman SS. Modeling of drug release from bulk-degrading polymers. Int J Pharm. 2011; 418(1):28–41. doi: 10.1016/j.ijpharm.2010.12.020 PMID: 21182912 17. Sackett CK, Narasimhan B. Mathematical modeling of polymer erosion: Consequences for drug delivery. Int J Pharm. 2011; 418(1):104–114. doi: 10.1016/j.ijpharm.2010.11.048 PMID: 21130849 18. Ford Versypt AN, Pack DW, Braatz RD. Mathematical modeling of drug delivery from autocatalytically degradable PLGA microspheres—A review. J Control Release. 2013; 165(1):29–37. doi: 10.1016/j. jconrel.2012.10.015 PMID: 23103455 19. Ford Versypt AN. Modeling of controlled-release drug delivery from autocatalytically degrading polymer microspheres. Ph.D. Thesis, University of Illinois at Urbana-Champaign. Urbana, IL; 2012. 20. Lyu S, Sparer R, Untereker D. Analytical solutions to mathematical models of the surface and bulk erosion of solid polymers. J Polym Sci, Part B: Polym Phys. 2005; 43(4):383–397. doi: 10.1002/polb. 20340 21. Antheunis H, van der Meer JC, de Geus M, Heise A, Koning CE. Autocatalytic equation describing the change in molecular weight during hydrolytic degradation of aliphatic polyesters. Biomacromolecules. 2010; 11(4):1118–1124. doi: 10.1021/bm100125b PMID: 20187614 22. Pitt CG, Schindler A. The kinetics of drug cleavage and release from matrices containing covalent polymer-drug conjugates. J Control Release. 1995; 33(3):391–395. doi: 10.1016/0168-3659(94)00113-9 23. Tzafriri AR. The kinetics of drug cleavage and release from matrices containing covalent polymer-drug conjugates. J Control Release. 2000; 63(1–2):69–79. 24. Wang Y, Pan J, Han X, Sinka C, Ding L. A phenomenological model for the degradation of biodegradable polymers. Biomaterials. 2008; 29(23):3393–3401. doi: 10.1016/j.biomaterials.2008.04.042 PMID: 18486970 25. Grizzi I, Garreau H, Li S, Vert M. Hydrolytic degradation of devices based on poly(DL-lactic acid) sizedependence. Biomaterials. 1995; 16(4):305–311. doi: 10.1016/0142-9612(95)93258-F PMID: 7772670 26. Fogler HS. Elements of Chemical Reaction Engineering. 4th ed. Upper Saddle River, NJ: Prentice Hall; 2006. 27. Deen WM. Analysis of Transport Phenomena. New York: Oxford University Press; 1998. 28. Estey T, Kang J, Schwendeman SP, Carpenter JF. BSA degradation under acidic conditions: A model for protein instability during release from PLGA delivery systems. J Pharm Sci. 2006; 95(7):1626–1639. doi: 10.1002/jps.20625 PMID: 16729268 29. Haberman R. Applied Partial Differential Equations: with Fourier Series and Boundary Value Problems. 4th ed. Upper Saddle River, NJ: Prentice Hall; 2004. 30. Edwards CH, Penney DE. Differential Equations and Boundary Value Problems: Computing and Modeling. 2nd ed. Upper Saddle River, NJ: Prentice Hall; 2000. 31. Schiesser WE. The Numerical Method of Lines: Integration of Partial Differential Equations. San Diego: Academic Press; 1991. 32. Schiesser WE. Partial Differential Equation Analysis in Biomedical Engineering: Case Studies with MATLAB. New York: Cambridge University Press; 2013. 33. Crank J. The Mathematics of Diffusion. 2nd ed. Oxford: Oxford University Press; 1975. 34. Fu K, Pack DW, Klibanov AM, Langer R. Visual evidence of acidic environment within degrading poly (lactic-co-glycolic acid) (PLGA) microspheres. Pharm Res. 2000; 17(1):100–106. doi: 10.1023/ A:1007582911958 PMID: 10714616 PLOS ONE | DOI:10.1371/journal.pone.0135506 August 18, 2015 14 / 14